## Topological Lifshitz Transitions and Fermi Arc Manipulation in Weyl Semimetal NbAs

H. F. Yang 1,2,3* , L. X. Yang 4* , Z. K. Liu 1,2* , Y. Sun 5* , C. Chen , H. Peng , M. Schmidt , 3 3 5 D. Prabhakaran 3 , B. A. Bernevig , C. Felser , B. H. Yan  and Y. L. Chen 6 5 7 1,2,3,4†

1 School of Physical Science and Technology, ShanghaiTech University, Shanghai 200031, P. R. China

2 ShanghaiTech Laboratory for Topological Physics, 200031 Shanghai, P. R. China

3 Department of Physics, University of Oxford, Oxford, OX1 3PU, UK

4 State Key Laboratory of Low Dimensional Quantum Physics and Department of Physics, Tsinghua

University, Beijing 100084, P. R. China

5 Max Planck Institute for Chemical Physics of Solids, D-01187 Dresden, Germany

6 Department of Physics, Princeton University, Princeton, New Jersey 08544, USA

7 Department of Condensed Matter Physics, Weizmann Institute of Science, Rehovot 7610001, Israel

* These authors contributed equally to this work

† Email: yulin.chen@physics.ox.ac.uk

Surface Fermi arcs (SFAs), the unique open Fermi-surfaces (FSs) discovered recently in topological Weyl semimetals (TWSs), are unlike closed FSs in conventional materials and can  give  rise  to  many  exotic  phenomena,  such  as  anomalous  SFA-mediated  quantum oscillations,  chiral  magnetic  effects,  three-dimensional  quantum  Hall  effect,  non-local voltage  generation  and  anomalous  electromagnetic wave transmission. Here, by using insitu surface decoration, we demonstrate successful manipulation of the shape, size and even the connections of SFAs in a model TWS, NbAs, and observe their evolution that leads to an unusual topological Lifshitz transition not caused by the change of the carrier concentration. The  phase  transition  teleports  the  SFAs  between  different  parts  of  the  surface  Brillouin zone. Despite the dramatic surface evolution, the existence of SFAs is robust and each SFA remains tied to a pair of Weyl points of opposite chirality, as dictated by the bulk topology.

## Introduction

Fermi-surfaces are boundaries of electronic bands in reciprocal space that separate occupied and unoccupied states. The  shape  and  volume  of  FSs  determine  the  electric,  magnetic,  optical  and even thermal properties of materials. In conventional materials, FSs form closed shapes, such as closed curves in two-dimensional (2D) electronic systems or closed surfaces in three-dimensional (3D) electronic systems. However, this orthodoxy was recently upended by the theoretical and experimental discovery of a new type of quantum state - the topological Weyl semimetal (TWS), in which open FSs - surface Fermi arcs (SFAs) - emerge 1-5 .

In  a  TWS,  linearly  dispersive  bulk  conduction  and  valence  bands  reminiscent  of  the dispersion of massless particles touch at an even number of Weyl points 1-5 (see  Fig.  1a,  where Weyl points in momentum space resemble magnetic monopoles). In a TWS, each Weyl point is associated  with  a  positive  or  negative  chirality.  On  the  surface  of  a  TWS,  exotic  topological surface states whose Fermi surfaces consist of open curves appear. The open curves are the SFAs that  must  originate  from  and  terminate  at  the  surface  projection  of  a  pair  of  Weyl  points  of opposite chirality 1-3 (see Fig. 1a).

The unusual SFAs and their interplay with bulk Weyl fermions can result in many exotic physical  phenomena,  such  as  anomalous  SFA-mediated  quantum  oscillations 6-9 (Fig.  1b),  the realization  of  chiral  magnetic  effects  (e.g.,  the  chiral  anomaly 10-13 and  the  universal  quantized contribution of SFAs  in  magneto-electric  transport 14 ), 3D  quantum  Hall  effect 15 , novel quasiparticle interference in tunnelling spectroscopy 16-19 ,  intriguing non-local voltage generation (Fig.  1c)  and  unusual  electromagnetic  wave  transmission 20-23 (Fig.  1d),  and  the  emergence  of Majorana modes when coupled with superconductivity 24 . Therefore, the capability of controlling and modifying the SFAs, especially the switching of SFAs between Weyl-points pairs (see Fig. 1a,  b),  are  naturally  desired  in  order  to  understand  and  manipulate  these  exciting  and  unusual phenomena.

In this work, by investigating the SFAs of NbAs, a model system from the transition-metal monophosphide (TMM) TWS family recently predicted and discovered 4,5,25-34 , we were able to directly manipulate the SFAs by surface decoration. Using in-situ monitoring with angle-resolved photoemission  spectroscopy  (ARPES),  for  the  first  time,  we  clearly  observe  the  evolution  of SFAs through an unusual topological transition where the SFAs switch the pairs of Weyl points they connect. Remarkably, despite the dramatic change of the shape and size of SFAs during the topological transition, each SFA remains connected to a pair of Weyl points (albeit different pairs before and after the transition) of opposite chirality, demonstrating the topological nature of the electronic structures of TWSs. Notably, this topological Lifshitz transition between open Fermi surfaces is not caused by the simple shift of the Fermi-energy due to the change of the carrier concentration;  rather,  it  is  caused  by  a  delicate  surface  modification  with  ordered  decoration atoms.  Furthermore,  the  Fermi  surface  consists  only  of  SFAs  unaccompanied  by  the  kinds  of topologically trivial states that are commonly observed in this family compounds 25-33 . The method to  control  and  manipulate the topological electronic states  of TWSs in this  work will  not  only open  a  new  frontier  for  the  exploration  of  fundamental  physical  phenomena  but  also  make possible the design of unusual electronic applications mediated by SFAs.

## Results

Basic  characterization  of  NbAs  crystals. NbAs  crystallizes  into  a  body-centred  tetragonal structure without inversion symmetry 35 , with four Nb-As layers in a unit cell stacking along the c direction (Fig. 1e). The crystal can be naturally cleaved between two adjacent Nb-As layers to yield a flat (001) surface ideal for ARPES measurements. As proposed by calculations 4,5,34 , there are 12 pairs of Weyl points in the Brillouin zone (BZ) connected by the SFAs (Fig. 1f), which is similar  to  other  TWSs  in  the  same  family 25-29,31 . The  high-quality  NbAs  crystals  (Fig.  1g) synthesized  for  this  work  show  sharp  X-ray  diffraction  patterns  along  all  three  crystalline orientations, and large, mirror-like flat surfaces that facilitate the ARPES measurements. Similar

to other recent reports 27,29 , in order to focus on the surface states, we utilize low-energy photons (e.g.  56  eV)  to  maximize  the  surface  sensitivity  and  increase  the  energy  and  momentum resolutions 36 .

Band structure of pristine surface. The electronic structure of pristine, freshly cleaved NbAs (Fig.  2a,  c)  show  the  characteristic  cross-shaped  FS  that  consists  of  spoon-  and  bowtie-like surface  FS  pockets  similar  to  other  TWS  compounds  of  the  same  family 25-29,31-33 .  These  FSs, whose surface nature is confirmed by photon-energy dependent ARPES measurements (see Fig. 2f  and  Supplementary  Figure 2 and 3  for details) and extensively discussed in recent works 30 , agree  well  with  our ab-initio calculations  of  surface  states  on  the  As-terminated  (001)  surface (Fig. 2b). These calculations confirm the connection pattern of the SFAs as sketched in Fig. 2d.

Figure-8-like  SFAs  emerging  on  potassium  decorated  surface. To  modify  the  SFAs  and examine their topological character,  we decorated  the  sample  surface by in-situ potassium  (K) deposition 37-39 .  On  one  hand,  surface  decoration  is  an  effective  method  to  disrupt  the  normal (trivial) surface states by changing the surface environments and introducing new surface Fermi surfaces. On the other hand, as the SFAs are protected by the topology of the bulk band structures, which  cannot  be  altered  by  surface  modification,  they  have  to  remain  even  after  surface decoration. Remarkably, after the surface decoration, a completely different FS emerged (Fig. 2g, i). The surface origin of the changing FS can be confirmed by photon-energy dependent ARPES measurements (see Fig. 2l, and Supplementary Figure 4 and 5). Compared to the pristine FS in Fig.  2a  and  2c,  the  new  FS  differs  not  only  in  the  size,  but  also  the  shape  and  the  connection pattern of each FS pieces.

In order to understand this change, and to make connection with the experimental data, we carried  out ab  initio calculations  to  simulate  the  surface  decoration  process  (Supplementary Figure  9  and  Supplementary  Note  2).  The  results  (Fig.  2h,  from  a  K-covered  NbAs  surface)

reproduce the figure-8-like surface FS that agrees excellently with the experimental results (Fig. 2i).  Interestingly,  the  calculations  also  show  that  the  FSs  now  consist  of  two  SFAs  with  a topologically different connection pattern to the Weyl points: unlike the pristine surface where the  spoon-like  SFAs  connect  the  adjacent  WPs  (Fig.  2d)  within  the  same  BZ,  the  SFAs  after decoration now even connect WPs from different BZs (see Fig. 2j). This is a manifestation of a topological quantum phase transition. Remarkably, despite the dramatic change of their shape and size, the SFAs still abide by the rule that each SFA must initiate and terminate at Weyl points of opposite chirality, as shown by stacking-plots of measured surface FSs and bulk dispersions with their momentum aligned in Fig. 2e and 2k. This clearly demonstrates the topological robustness of the SFAs (bulk states measurements and detailed discussion can be found in Supplementary Note 4).

Furthermore,  unlike  the  pristine  surface  where  the  FS  consists  of  both  SFAs  (marked  as SFAs) and conventional surface states (e.g. the bowtie-like surface states, marked as Trivial SS in Fig. 2a, 2c and previous works 25-29, 31-33 ), the FS after the surface decoration also shows a much simpler structure, which only consists of two long SFAs without other surface states (Fig. 2g, i) and makes it the cleanest system of Fermi-arcs observed to date. This simplicity, as well as the rather  large  length  of  SFAs,  will  help  realize  SFA-related  phenomena  (e.g.  novel  quantum oscillations,  non-local  transport,  quasiparticle  interference  in  tunneling  spectroscopy,  Majorana modes, etc.) without the spurious effects of trivial surface states.

In addition to the FSs, the difference between surface electronic structures before and after the surface modification can be seen in other aspects of the electronic structure, such as the band dispersions  and  the  evolution  of  the  constant  energy  contours,  as  demonstrated  in  Fig.  3.  The accumulation of the dosed K atoms on the sample surface can be clearly seen by the characteristic K 3p level,  which  is  absent  on  the  pristine  surface  (Fig.  3a)  but  emerges  after  the  surface decoration (Fig. 3e). Associated with the surface modification, we summarize the overall band structure in volume plots (Fig. 3b, f), the high-symmetry band dispersions across the whole BZ

(Fig. 3c, g), and the evolution of band contours at different binding energies (Fig. 3d, h). Notably, the side-by-side comparisons of our comprehensive electronic structures studies show excellent agreement with the surface states' band structure results from our ab initio calculations.

Besides the agreement of the general band structure, in Fig. 4 the fine structure of the figure8-like FS is further resolved. 2D curvature analysis 40 results (Fig. 4b), Fermi contours at higher binding energies (like EB = 0.1 eV in Fig. 4d), and band dispersions for cuts through the figure-8 showing four band crossings of the topological surface states (TSSs) (Fig. 4e), consistently reveal that  the  figure-8-like  FS  is  composed  of  two  long  SFAs,  and  confirms  their  connectivity  to projections of Weyl points as predicted (Fig. 4c).

Topological  quantum  Lifshitz  transition. To  investigate  the  evolution  of  the  SFAs  and  its topological phase transition, we carried out detailed K-dose dependent measurements of the band structure, as illustrated in Fig. 5. The overall evolution constitutes of two stages: Stage I is from Panel a - c and Stage II is from d - f of Fig. 5. Within each stage, the surface band structure including the FS and dispersion evolve continuously and show only quantitative changes (such as the continuously shrinking of the spoon- and bowtie-like FS pockets in Stage I and the growing of the figure-8-like FS pieces in Stage II). However, between the two stages, a topological quantum Lifshitz transition (TQLT) occurs, manifested by the dramatic change of the FS topology and the band dispersions, which is concomitantly accompanied by the disappearance of the bowtie-like trivial SSs in stage I, leaving only the SFAs of Stage II. Such a transition cannot be explained by a simple rigid band shift of EF, as is also confirmed by our ab initio calculations (more details can be found in Supplementary Note 2). Further orbital calculations show that while the TSS of the pristine surface harbours a complicated multi-orbital contributions from both As and Nb, the TSS of K-decorated is dominated by Nb d z 2 orbital (Supplementary Figure 8).

## Discussion

We  have  proved  the  capability  of  direct  manipulation  of  the  SFAs  and  the  control  of  their topological character: the topologically distinct connection patterns between the Weyl points. For the  first  time,  we  have  observed  a  Lifshitz  transition  of  an  open  Fermi  surface;  provided  an important, yet previously unobserved proof that Fermi arcs are topological; and shown how to change the topology of a surface Fermi arc. By varying the surface physical properties (e.g. the carrier  concentration),  we  provided  an  effective  method  to  investigate  the  unique  topological electronic structures of TWSs, with future work needed to explore more of their exotic physical phenomena and, possibly, unusual electronic applications.

## Methods

Synthesis  of  bulk  single  crystals. NbAs  single  crystals  were  synthesized  by  chemical  vapor transport using iodine as the transport agent. We first obtained a polycrystalline precursor, then grew single crystals from it. Precursor polycrystalline samples were prepared from a mixture of high-purity  (&gt;99.99%)  Nb  and  As  elements.  The  mixture  was  sealed  under  high  vacuum  in  a quartz tube, which was sealed in another evacuated tube for extra protection. First, the vessel was heated to 600°C at a rate of 50°C/hour. After 10 hours' soaking, it was slowly heated to 1050° C at  a  rate  of  30° /hour  and  then  kept  at  this  temperature  for  24  hours.  Finally  the  vessel  was C cooled  to  room  temperature.  From  the  resulting  polycrystalline  precursor,  single  crystals  were grown using chemical vapor transport in a two-zone furnace. The polycrystalline NbAs powder and  0.46  mg/cm 3 of  iodine  were  loaded  into  a  24-mm-diameter  quartz  tube  and  sealed  under vacuum. The charged part of the tube was kept at 1150° C and the other end was kept at 1000° C for three weeks. The resulting crystals with shiny mirror-like surfaces can be as large as 0.5 - 1.0 mm in size, suitable for standard high-resolution ARPES measurements.

Angle-resolved photoemission spectroscopy (ARPES). ARPES measurements were performed at  BL  I05  of  the  Diamond  Light  Source  (DLS),  UK.  Data  were  recorded  by  a  Scienta  R4000 analyzer.  The  measurement  sample  temperature  and  pressure  were  10  K  and  1.5× 10 -10 Torr, respectively.  The  overall  energy  and  angle  resolutions  were  15  meV  and  0.2 ,  respectively. ◦ Linearly horizontally polarized (LH) photons are used as they show high intensity with all band structure features  being  clearly  captured.  Fresh  NbAs  surfaces  for  ARPES  measurements  were obtained  by  cleaving  in-situ  the  crystals  at  low  temperatures  (10  K).  Potassium  atoms  were evaporated in-situ onto cleaved (001) NbAs surfaces by a commercial SAES potassium dispenser

under an ultrahigh vacuum of 2.0× 10 -10 Torr.

ab  initio calculations. Electronic  structures  were  calculated  by  the  density-functional  theory (DFT) method which is implemented in the Vienna ab initio Simulation Package (VASP) 41 . The core  electrons  were  represented  by  the  projected  augmented  wave  method 42 .  The  exchangecorrelation  was considered in the generalized gradient approximation (GGA) 43 and  spin-orbital coupling (SOC) was included self-consistently. The energy cut off was set to be 300 eV for the plane-wave basis. Experimental lattice parameters were used in the construction of a model slab with a thickness of seven unit cells to simulate a surface, in which the top and bottom surfaces are terminated  by  As  and  Nb,  respectively.  Positions  of  outermost  four  atomic  layers  were  fully optimized to consider surface atomic relaxation. The surface band structures and Fermi surfaces were projected onto the first unit cell of the As-terminated side, which fit the experimental band structure well. We adopted 12× 12 and 400× 400 k-point grids in the self-consistent charge and in the Fermi surface calculations, respectively.

Data  availability. The  data  generated  and  analysed  during  this  study  are  available  from  the corresponding author  upon request.

## References

- 1. Wan, X., Turner, A. M., Vishwanath, A. &amp; Savrasov, S. Y. Topological semimetal and Fermiarc surface states in the electronic structure of pyrochlore iridates. Phys. Rev. B 83 ,  205101 (2011).
- 2.  Burkov,  A. A.,  Hook,  M. D. &amp; Balents, L. Topological nodal semimetals. Phys. Rev. B 84 , 235126 (2011).
- 3. Balents, L. Weyl electrons kiss. Physics 4 , 36 (2011).
- 4.  Weng,  H.  M.,  Fang,  C.,  Fang,  Z.,  Bernevig,  B.  A.  &amp;  Dai,  X.  Weyl  semimetal  phase  in noncentrosymmetric transition-metal monophosphides. Phys. Rev. X 5 , 011029 (2015).
- 5. Huang S. -M. et al. A Weyl Fermion semimetal with surface Fermi arcs in the transition metal monopnictide TaAs class. Nat. Commun. 6 , 7373 (2015).
- 6. Potter, A. C., Kimchi, I. &amp; Vishwanath, A. Quantum oscillations from surface Fermi arcs in Weyl and Dirac semimetals. Nat. Commun . 5 , 5161 (2014).
- 7. Bulmash, D. &amp; Qi, X. -L. Quantum oscillations in Weyl and Dirac semimetal ultrathin films. Phys. Rev. B 93 , 081103(R) (2016).
- 8.  Zhang,  Y.,  Bulmash,  D.,  Hosur,  P.,  Potter,  A.  C.  &amp;  Vishwannath,  A.  Quantum  oscillations from generic surface Fermi arcs and bulk chiral modes in Weyl semimetals. Sci. Rep. 6 , 23741 (2016).
- 9. Moll, P. J. W. et al. Transport evidence for Fermi-arc-mediated chirality transfer in the Dirac semimetal Cd3As2. Nature 535 , 266-270 (2016).
- 10.  Zyuzin,  A.  A.  &amp;  A.  A.  Burkov.  Topological  response  in  Weyl  semimetals  and  the  chiral anomaly. Phys. Rev. B 86 , 115133 (2012).
- 11. Liu, C. -X., Ye, P. &amp; Qi, X. -L. Chiral gauge field and axial anomaly in a Weyl semimetal. Phys. Rev. B 87 , 235306 (2013).
- 12. Huang X. et al . Observation of the chiral-anomaly-induced negative magnetoresistance in 3D Weyl semimetal TaAs. Phys. Rev. X 5 , 031023 (2015).

- 13. Zhang, C. -L. et al . Signatures of the Adler -Bell -Jackiw chiral anomaly in a Weyl fermion semimetal. Nat. Commun. 7 , 10735 (2016).
- 14. Baireuther, P., Hutasoit, J. A., Tworzydlo, J. &amp; Beenakker, C. W. J. Scattering theory of the chiral magnetic effect in a Weyl semimetal: interplay of bulk Weyl cones and surface Fermi arcs. New J. Phys. 18 , 045009 (2016).
- 15. Wang, C. M., Sun, H. -P., Lu, H. -Z. &amp; Xie, X. C. 3D quantum Hall effect of Fermi arcs in topological semimetals. Phys . Rev  Lett . . 119 , 136806 (2017).
- 16. Kourtis, S., Li, J., Wang, Z., Yazdani, A. &amp; Bernevig, B. A. Universal signatures of Fermi arcs  in  quasiparticle  interference  on  the  surface  of  Weyl  semimetals. Phys.  Rev.  B 93 , 041109(R) (2016).
- 17. Inoue, H. et al . Quasiparticle interference of the Fermi arcs and surface-bulk connectivity of a Weyl semimetal. Science 351 , 1184-1187 (2016).
- 18. Batabyal, R. et al . Visualizing weakly bound surface Fermi arcs and their correspondence to bulk Weyl fermions. Sci. Adv. 2 , e1600709 (2016).
- 19. Hosur, P. Friedel oscillations due to Fermi arcs in Weyl semimetals. Phys. Rev. B 86 , 195102 (2012).
- 20. Parameswaran, S. A., Grover, T., Abanin, D. A., Pesin, D. A. &amp; Vishwanath, A. Probing the chiral anomaly with nonlocal transport in three-dimensional topological semimetals. Phys. Rev. X 4 , 031035 (2014).
- 21.  Baum,  Y.,  Berg,  E.,  Parameswaran,  S.  A.  &amp;  Stern,  A.  Current  at  a  distance  and  resonant transparency in Weyl semimetals. Phys. Rev. X 5 , 041046 (2015).
- 22. Ishizuka, H., Hayata, T., Ueda, M. &amp; Nagaosa, N. Emergent electromagnetic induction and adiabatic  charge  pumping  in  noncentrosymmetric  Weyl  semimetals. Phys.  Rev.  Lett . 117 , 216601 (2016).
- 23. Rosenstein, B., Kao, H. C. &amp; Lewkowicz, M. Nonlocal electrodynamics in Weyl semimetals. Phys. Rev. B 95 , 085148 (2017).
- 24.  Baireuther,  P.,  Tworzydlo,  J.,  Breitkreiz,  M.,  Adagideli,  I.  &amp;  Beenakker,  C.  W.  J.  WeylMajorana solenoid. New J. Phys. 19 , 025006 (2017).
- 25. Lv, B. Q. et al. Observation of Weyl nodes in TaAs. Nat. Phys. 11 , 724-727 (2015).
- 26. Xu, S. -Y. et al. Discovery of a Weyl fermion semimetal and topological Fermi arcs. Science 349 , 613-617 (2015).
- 27. Yang, L. X. et al . Weyl semimetal phase in the non-centrosymmetric compound TaAs. Nat. Phys. 11 , 728-732 (2015).
- 28. Lv, B. Q. et  al. Experimental discovery of Weyl semimetal TaAs. Phys. Rev. X 5 ,  031013 (2015).
- 29. Liu, Z. K. et  al. Evolution of the Fermi surface of Weyl semimetals in the transition metal pnictide family. Nat. Mater. 15 , 27-31 (2015).
- 30. Xu, S. -Y. et al . Discovery of a Weyl fermion state with Fermi arcs in niobium arsenide. Nat. Phys. 11 , 748-754 (2015).
- 31.  Xu,  D.  -F. et  al. Observation  of  Fermi  arcs  in  non-centrosymmetric  Weyl  semi-metal candidate NbP. Chin. Phys. Lett. 32 , 107101 (2015).
- 32. Souma, S. et al . Direct observation of nonequivalent Fermi-arc states of opposite surfaces in the noncentrosymmetric Weyl semimetal NbP. Phys. Rev. B 93 , 161112(R) (2016).
- 33. Xu, N. et al . Observation of Weyl nodes and Fermi arcs in tantalum phosphide. Nat. Commun. 7 , 11006 (2016).
- 34. Sun,  Y.,  Wu,  S.  -C.  &amp;  Yan, B.  Topological  surface  states  and  Fermi  arcs  of  the noncentrosymmetric Weyl semimetals TaAs, TaP, NbAs, and NbP. Phys. Rev. B 92 , 115428 (2015).
- 35. Boller, H. &amp; Parthe  E. The transposition structure of NbAs and of similar monophosphides , and arsenides of niobium and tantalum. Acta Crystallogr. 16 , 1095-1101 (1963).

- 36.  Damascelli,  A.,  Hussain,  Z.  &amp;  Shen,  Z.  X.  Angle-resolved  photoemission  studies  of  the cuprate superconductors. Rev. Mod. Phys. 75 , 473-541 (2003).
- 37. Hossain, M. A. et al. In situ doping control of the surface of high-temperature superconductors. Nat. Phys. 4 , 527-531 (2008).
- 38.  Liu,  Z.  K. et  al. Discovery  of  a  three-dimensional  topological  Dirac  semimetal,  Na3Bi. Science 343 , 864-867 (2014).
- 39. Liu, Z. K. et al. A stable three-dimensional topological Dirac semimetal Cd3As2. Nat. Mater. 13 , 677-681 (2014).
- 40. Zhang, P. et al . A precise method for visualizing dispersive features in image plots. Rev. Sci. Instrum . 82 , 043712 (2011).
- 41. Kresse, G. &amp; Furthmü ller, J. Effcient iterative schemes for ab initio total-energy calculations using a plane-wave basis set. Phys. Rev. B 54 , 11169-11186 (1996).
- 42. Blö chl, P. E. Projector augmented-wave method. Phys. Rev. B 50 , 17953-17979 (1994).
- 43. Perdew, J. P., Burke, K. &amp; Ernzerhof, M. Generalized gradient approximation made simple. Phys. Rev. Lett. 77 , 3865-3868 (1996).

## Acknowledgements

We thank John A. McGuire for polishing the writing of this paper. This work was supported by the National Key R&amp;D program of China (No. 2017YFA0305400), the National Natural Science Foundation  of  China  (Grants  No.  11774190,  No.  11674229  and  No.  11634009).  Y.L.C. acknowledges insightful discussion with Siddharth Parameswaran and the support of the EPSRC Platform Grant (Grant No EP/M020517/1) and Hefei Science Center CAS (2015HSC-UE013). Y.L.C.  and  L.X.Y.  acknowledge  the  support  from  Tsinghua  University  Initiative  Scientific Research  Program.  B.A.B.  acknowledges  an  early  discussion  with  Ady  Stern  in  Banff,  2015, where he was introduced to the idea of changing the Fermi arc topology of a Dirac semimetal. B.A.B. was supported by Department of Energy de-sc0016239, Simons Investigator Award, the Packard Foundation, and the Schmidt Fund for Innovative Research, NSF EAGER grant DMR1643312,  ONR-N00014-14-1-0330,  ARO  MURI  W911NF-  12-1-0461,  NSF-MRSEC  DMR1420541. C.F. acknowledges financial support by the ERC Advanced Grant (No 291472 'Idea Heusler').  B.Y.  is  supported  by  a  research  grant  from  the  Benoziyo  Endowment  Fund  for  the Advancement  of  Science  and  by  a  Grant  from  the  German-Israeli  Foundation  for  Scientific Research and Development (GIF Grant no. I-1364-303.7/2016). H.F.Y. acknowledges financial support from the China Postdoctoral Science Foundation (Grant No. 2017M611635).

## Author contributions

Y.L.C. conceived the experiments. H.F.Y., L.X.Y. and Z.K.L. carried out ARPES experiments with  the  assistance  of  C.C.  and  H.P.  M.S.,  D.P.  and  C.F.  synthesized  and  characterized  bulk single  crystals.  Y.S.  and  B.H.Y.  performed ab  initio calculations.  B.A.B  contributed  to  the scientific discussion and revision of the paper.

## Additional information

Competing interests: The authors declare no competing interests.

Figure 1 | Topological Lifshitz transition of SFAs and characterization of NbAs crystals. a ,

![image](https://ac.marcodsn.me/arxiv-markdown-images/1908.01155v1-figure-bf2cd680-560f-464d-9fb8-b9cc6d6ed819.jpg)

Sketch of topological Lifshitz transition of SFAs in TWSs. Balls and green crescents represent Weyl points and  Fermi  arcs,  respectively. b ,  Schematic  illustration  of  Weyl  orbits  that  weave together  chiral  bulk  states  and  SFAs  of  top  and  bottom  surfaces  in  magnetic  fields.  When  a topological  Lifshitz  transition  of  SFAs  occurs  at  the  top  surface,  the  Weyl  orbits  and  relevant quantum  phenomena  change,  thus  modifying  the  physical  responses  of  TWSs. c ,  Schematic illustration of non-local voltage generation 21 . d , Schematic illustration of unusual electromagnetic wave transmission 21 . e, Sketch of the NbAs crystal structure, showing a body-centered-tetragonal structure without inversion symmetry. f ,  Bulk and projected surface Brillouin zones (BZs) with Weyl points connected by surface Fermi arcs. g , Optical image of a typical NbAs crystal and Xray diffraction patterns along the (001), (010), and (100) crystalline directions.

Figure  2  |  Fermi  surface  comparison  of  pristine  and  potassium  (K)-decorated  NbAs. a ,

![image](https://ac.marcodsn.me/arxiv-markdown-images/1908.01155v1-figure-f724bee0-637a-4314-813f-19909aefa068.jpg)

Fermi surface of pristine NbAs consisting of SFAs and trivial surface states (marked as Trivial SS). b c -are  the  calculated  and  measured  Fermi  surface  around the X  point, respectively. ̅ d , Sketch  of  the  SFAs'  connectivity  to  projections  of  Weyl  points. e ,  In  pristine  NbAs,  SFAs connect projections of bulk Weyl points (upper image: surface Fermi surface showing the SFAs; lower image: bulk Weyl dispersions with overlaid calculated bulk dispersion). f , two representative Fermi surfaces measured with 144 and 172 eV photons show spoon- and bowtielike features of almost identical size, thus revealing their surface nature. g ,  Figure-8-like Fermi surface of K-decorated NbAs consisting of long SFAs without trivial surface states. The overlaid yellow  arrows  show  that  the  figure-8-like  FS  splits  into  two  branches  near  kx=  0  and  ky  =  0 regions. h i -  are the calculated and measured Fermi surface around the  point, respectively, which show good agreement.  , The SFAs and connection pattern are schematically displayed. j k , In Kdecorated  NbAs,  SFAs  connect  projections  of  bulk  Weyl  points  (upper  image:  surface  Fermi surface  showing  the  SFAs;  lower  image:  bulk  Weyl  dispersions  with  overlaid  calculated  bulk dispersion). i ,  Two  representative  Fermi  surfaces  measured  with  80  and  96  eV  photons,  show figure-8-like  features  of  almost  identical  size,  thus  revealing  their  surface  nature.  Horizontally polarized  photons  are  used  as  they  produce  high  intensity  signals  and  clearly  reveal  all  band structure  features.  (Note  that  the  color  scale  of  the  calculated  bands  represent  their  surface

projection,  i.e.  the  bold  red  curves  represent  the  surface  states  while  the  faded  red  curves represent bands with strong bulk origin).

![image](https://ac.marcodsn.me/arxiv-markdown-images/1908.01155v1-figure-020582d0-a2d2-4813-b2bc-db6574c557a8.jpg)

Figure 3 | Measured and calculated band structures of pristine and K-decorated NbAs. a ,

![image](https://ac.marcodsn.me/arxiv-markdown-images/1908.01155v1-figure-b5f58625-0c93-4ce3-ab10-9bccaf60f51b.jpg)

![image](https://ac.marcodsn.me/arxiv-markdown-images/1908.01155v1-figure-282c440a-2b10-47cc-b123-a791696cd45e.jpg)

![image](https://ac.marcodsn.me/arxiv-markdown-images/1908.01155v1-figure-df93a8b4-fb5b-47c5-aea7-7bae4a416c1a.jpg)

![image](https://ac.marcodsn.me/arxiv-markdown-images/1908.01155v1-figure-0ca1db02-9465-47b8-8ae3-8547b3c6ab83.jpg)

![image](https://ac.marcodsn.me/arxiv-markdown-images/1908.01155v1-figure-f47b8c03-e3fe-4faa-883f-0a112d9488f9.jpg)

![image](https://ac.marcodsn.me/arxiv-markdown-images/1908.01155v1-figure-28e27598-7d14-4f10-ab38-b77e90fd1675.jpg)

![image](https://ac.marcodsn.me/arxiv-markdown-images/1908.01155v1-figure-593c5148-dccf-4940-ab89-03f5776bc78f.jpg)

Core-level photoemission spectrum of cleaved NbAs (001) surface (pristine), clearly showing the characteristic As and Nb peaks. b ,  3D  intensity  plot  of  the  band  structure  illustrating  the  band dispersions. c ,  Excellent  agreement  between  measured  and  calculated  band  dispersions  along high-symmetry directions with trivial surface states (Trivial SSs) and topological surface states (TSSs generating SFAs) marked. d , Side-by-side comparison between experiments and calculations, which exhibits good agreement, of three representative constant-energy contours (Eb = 0, 0.15, 0.30 eV). For comparison, these contours are obtained by mirroring the photoemission spectrum with respect to  the  ky  axis. e ,  Core-level  photoemission  spectrum  of  K-dosed  NbAs, which clearly displays the K 3p peak, and pristine NbAs.   f h : same as b -d but displaying the band structures of K-decorated NbAs. Our measured data agree well with the calculations. In g , Cyan arrows mark band crossings of the TSSs (corresponding to SFAs). (Note that the color scale

of the calculated bands represent their surface projection, i.e. the bold red curves represent the surface states while the faded red curves represent bands with strong bulk origin).

Figure 4 | Resolving the fine structure of figure-8-like FS. a-c are the measured Fermi surface patch around the  X  point, 2D curvature analysis results and calculations, respectively. Nominal ̅ K dosage for this set of data is 1.8 monolayer (ML), which is slightly smaller than that of the Kdosed data presented in Figs. 2 and 3. d , Measured constant-energy contour at 0.1 eV below EF. e , Three  representative  band  dispersions  along  cut  #1,  #2,  and  #3,  clearly  showing  four  band crossings of the TSSs that leads to two long SFAs forming the figure-8-like FS.

![image](https://ac.marcodsn.me/arxiv-markdown-images/1908.01155v1-figure-10776776-61b6-4365-b807-47204845b4ef.jpg)

Figure 5 | Detailed band structure evolution of topological Lifshitz transition of SFAs. a -f ,

![image](https://ac.marcodsn.me/arxiv-markdown-images/1908.01155v1-figure-e58e0cfb-95f2-490b-914d-753a7fb8f78f.jpg)

g ,  and h are  the  evolution  of  the  FS,  representative  band  dispersion  along  the M ̅ - ̅ Y - M ̅ direction, and 3D intensity plot of the overall band structure with progressively increasing the K dose, respectively. For comparison, these contours are obtained by mirroring the photoemission spectrum with respect to the ky axis. The overall evolution consists of two stages: Stage I is from Panel a to Panel c , and Stage II is from Panel d to Panel f . Between these two stages, a surface topological quantum Lifshitz transition (TPLT) occurs. We note that the uneven intensity of the FS between the first and second BZs are due to the photoemission matrix element effect 36 .
H. F. Yang L. X. Yang Z. K. Liu Y. Sun C. Chen H. Peng M. Schmidt D. Prabhakaran B. A. Bernevig C. Felser B. H. Yan Y. L. Chen
Topological Lifshitz Transitions and Fermi Arc Manipulation in Weyl Semimetal NbAs
Surface Fermi arcs (SFAs), the unique open Fermi-surfaces (FSs) discovered
recently in topological Weyl semimetals (TWSs), are unlike closed FSs in
conventional materials and can give rise to many exotic phenomena, such as
anomalous SFA-mediated quantum oscillations, chiral magnetic effects,
three-dimensional quantum Hall effect, non-local voltage generation and
anomalous electromagnetic wave transmission. Here, by using in-situ surface
decoration, we demonstrate successful manipulation of the shape, size and even
the connections of SFAs in a model TWS, NbAs, and observe their evolution that
leads to an unusual topological Lifshitz transition not caused by the change of
the carrier concentration. The phase transition teleports the SFAs between
different parts of the surface Brillouin zone. Despite the dramatic surface
evolution, the existence of SFAs is robust and each SFA remains tied to a pair
of Weyl points of opposite chirality, as dictated by the bulk topology.